Recent Advances in Inorganic Nanomaterials Synthesis Using Sonochemistry: A Comprehensive Review on Iron Oxide, Gold and Iron Oxide Coated Gold Nanoparticles

Sonochemistry uses ultrasound to improve or modify chemical reactions. Sonochemistry occurs when the ultrasound causes chemical effects on the reaction system, such as the formation of free radicals, that intensify the reaction. Many studies have investigated the synthesis of nanomaterials by the sonochemical method, but there is still very limited information on the detailed characterization of these physicochemical and morphological nanoparticles. In this comprehensive review, recent advances in the sonochemical synthesis of nanomaterials based on iron oxide nanoparticles (Fe3O4NP), gold nanoparticles (AuNP) and iron oxide-coated gold nanoparticles (Fe3O4@Au NP) are discussed. These materials are the most studied materials for various applications, such as medical and commercial uses. This review will: (1) address the simple processing and observations on the principles of sonochemistry as a starting point for understanding the fundamental mechanisms, (2) summarize and review the most relevant publications and (3) describe the typical shape of the products provided in sonochemistry. All in all, this review’s main outcome will provide a comprehensive overview of the available literature knowledge that promotes and encourages future sonochemical work.


Introduction
Reducing the material's size to the nanoscale limits the electrons inside to a small space that changes its physicochemical properties [1]. Such an expedited transition has given rise to many new applications while enhancing existing ones. The idea of synthesizing nanomaterials with the appropriate morphology and applicable properties has therefore stimulated great interest in this technological evolution. Through simple solution-based approaches such as hydrothermal, solvothermal and sonochemistry to cutting-edge approaches as ablation, epitaxy and lithography, the diversity of nanomaterial synthesis techniques can be exploited to monitor their development. Sonochemistry provides a special crystallinity control that enables the preparation of amorphous metals, metal alloys and metal oxide [2]. Compared to most approaches, sonochemical is very economical, allowing individual enthusiasts and researchers to experience and try out ideas [3]. It has grown to prominence with a rise in interest in material processing and engineering over the last 30-40 years. Nonetheless, the study of chemical solutions and chemical reactions with the use of sonochemical dates back to the early 20th century [4]. Physical methods such as vapor deposition, plasma glow discharge and gas-phase sputtering are prohibitively costly, whereas chemical methods such as electrolysis, photochemical synthesis and electroreduction yield greater nanoparticle sizes and have problems with mass processing. A third technique, such as the sonochemical process, solved some of the drawbacks described above by generating nanoparticles of smaller sizes [5]. The microwave method H 2 , and these resulting strong oxidants and reductants, in turn, are employed during different reactions of the sonochemical in the aqueous solutions [17].
For Fe 3 O 4 NPs, For AuNPs, the formation of the AuNPs takes into account the fact that free radical species are produced by the ultrasonic irradiation of water molecules (Equation (7)).
Au + + 2e → Au 0 The formation of Fe 3 O 4 NPs@AuNPs and the sonochemistry mechanism for coating the Fe 3 O 4 surface by Au NPs were discussed in detail in our previous work [32]. Briefly, sodium citrate can activate the reaction of the Fe 3 O 4 surface with carboxylate ions (-COO − ), which enables the strong coordination of highly -COO − water with the Fe atom of Fe 3 O 4 NPs. The mechanism that controls the bonding of Au NPs to the Fe 3 O 4 surface is linked to the microjets and shock waves generated within the vicinity of surfaces of the solid, following the bubble collapse [33]. These microjets initiate the sintering of micrometersized metallic particles and drive the NPs in the direction of the Fe 3 O 4 surface at very high velocities [33]. The jets react with free carboxylate ions (-COO − ) on the Fe 3 O 4 surface, resulting in Au nanoshell formation on the Fe 3 O 4 surface.

Nanomaterial Ultrasonic Synthesis
Fe 3 O 4 NPs, AuNPs and Fe 3 O 4 @AuNPs are the main materials of interest due to their biocompatibility, unique superparamagnetic properties, chemical stability, oxidation resistance and optical properties and which are important for fields such as catalysis and biomedical applications [34][35][36]. Ultrasound irradiation has recently been widely used in the synthesis of nanomaterials [37]. As clarified, high-intensity ultrasound results primarily in acoustic cavitation [38], which, in turn, initiates a distinctive interface between energy and matter [39]. This enables a wide range of chemical reactions and the production of a range of exceptional nanostructured materials [17]. Acoustic cavitation dynamics depend on the localized environment, either a uniform liquid or an inhomogeneous interface between a solid and liquid. For homogenous liquids that produce spherical cavities, acoustic cavitation produces implosive bubbles and waves, generating higher pressure with amplitudes above 10 kbar [40]. Conversely, the acoustic cavitation is asymmetric for an inhomogeneous medium and is related to high-speed microjets that influence the solid surface, causing mechanical damage [41]. The collapsing bubble's potential energy is converted into the microjet's kinetic energy with speeds of 100 s of m/s. Nonetheless, Doktycz and Suslick announced that solid particles under the collapsing bubble diameter (~150 µm) unable to start a microjet formation after an ultrasonic field of 2 kHz were irradiated [42]. Alternatively, traditional cavitation and shock wave emissions occurred [43].

Fe 3 O 4 NPs
Fe 3 O 4 NPs can easily be synthesized using a sonochemical method via very high pressures and temperatures generated by ultrasonic irradiation by decomposing iron salts and other nanostructures from an inorganic iron precursor [44]. The ultrasonic irradiation generates high temperatures that lead to the formation of Fe 3 O 4 NPs through the decomposition of iron salts [45]. Fe 3 O 4 NPs improved their hydrophilic and monodisperse properties through the ultrasonic irradiation process [46,47]. Many authors have recently reported using a sonochemical way to synthesize Fe 3 O 4 with promising physicochemical properties, such as a high surface area and high electron storage ability [48,49].
Zuzana and Kerstin synthesized Fe 3 O 4 NPs and coated them with dextran as a capping agent [50]. The larger cavitation bubbles at lower frequencies release more energy and create exceptional reaction conditions concerning pressure and temperature, further facilitating the development of the larger magnetite cores. This method has several advantages, such as a high chemical reaction rate, high yields and cost-effective synthesis. Sriram et al. reported a rapid and straightforward fabrication of Fe 3 O 4 NPs decorated by graphene oxide (GOS) by the sonochemical method [51]. This process involves a GOS ultrasound-assisted reduction reaction. Furthermore, the advantages of the modified Fe 3 O 4 NPs decorated by GOS were its reproducibility, repeatability and high stability. Figure 1a,b presented TEM and SEM images of Fe 3 O 4 NPs decorated by GOS. The nanoparticles have a spherical shape with a size of about 96 nm (Table 1). [42]. Alternatively, traditional cavitation and shock wave emissions occurred [43].

Fe3O4NPs
Fe3O4NPs can easily be synthesized using a sonochemical method via very high pressures and temperatures generated by ultrasonic irradiation by decomposing iron salts and other nanostructures from an inorganic iron precursor [44]. The ultrasonic irradiation generates high temperatures that lead to the formation of Fe3O4NPs through the decomposition of iron salts [45]. Fe3O4NPs improved their hydrophilic and monodisperse properties through the ultrasonic irradiation process [46,47]. Many authors have recently reported using a sonochemical way to synthesize Fe3O4 with promising physicochemical properties, such as a high surface area and high electron storage ability [48,49].
Zuzana and Kerstin synthesized Fe3O4NPs and coated them with dextran as a capping agent [50]. The larger cavitation bubbles at lower frequencies release more energy and create exceptional reaction conditions concerning pressure and temperature, further facilitating the development of the larger magnetite cores. This method has several advantages, such as a high chemical reaction rate, high yields and cost-effective synthesis. Sriram et al. reported a rapid and straightforward fabrication of Fe3O4NPs decorated by graphene oxide (GOS) by the sonochemical method [51]. This process involves a GOS ultrasound-assisted reduction reaction. Furthermore, the advantages of the modified Fe3O4NPs decorated by GOS were its reproducibility, repeatability and high stability. Figure 1a,b presented TEM and SEM images of Fe3O4NPs decorated by GOS. The nanoparticles have a spherical shape with a size of about 96 nm (Table 1). An ultrasonic-assisted coprecipitation approach of synthesizing magnetite nanoparticles was recorded by Villegas et al. [52]. This approach identified a 16-nm amphoteric crystallite size and provided a superparamagnetic behavior that separated less easily from a solution in 1 min by using only a magnet. Fe3O4NPs decorated on multi-wall nanotubes (MWCNTs) were successfully produced using a rapid and easy sonochemical process without any chemical treatment on MWCNTs [53]. Fe3O4@ MWCNTs displayed a uniform, fine nanoparticle distribution in the MWCNTs. Fe3O4@MWCNTs demonstrated an effective catalytic efficiency after 1 h of treatment with 20-mg/L persulfate. Fe3O4NPs helped produce sulfate radicals and hydroxyl radicals in the Fe3O4@ MWCNTs hybrid catalyst, whereas the size of the Fe3O4 clusters could affect the transmission of electrons for radical production. In addition, the combination of persulfate and Fe3O4@MWCNTs decreased the remaining cell number to 9.4% within 30 min of treatment using high-fre- An ultrasonic-assisted coprecipitation approach of synthesizing magnetite nanoparticles was recorded by Villegas et al. [52]. This approach identified a 16-nm amphoteric crystallite size and provided a superparamagnetic behavior that separated less easily from a solution in 1 min by using only a magnet. Fe 3 O 4 NPs decorated on multi-wall nanotubes (MWCNTs) were successfully produced using a rapid and easy sonochemical process without any chemical treatment on MWCNTs [53]. Fe 3 O 4 @ MWCNTs displayed a uniform, fine nanoparticle distribution in the MWCNTs. Fe 3 O 4 @MWCNTs demonstrated an effective catalytic efficiency after 1 h of treatment with 20-mg/L persulfate. Fe 3 O 4 NPs helped produce sulfate radicals and hydroxyl radicals in the Fe 3 O 4 @ MWCNTs hybrid catalyst, whereas the size of the Fe 3 O 4 clusters could affect the transmission of electrons for radical production. In addition, the combination of persulfate and Fe 3 O 4 @MWCNTs decreased the remaining cell number to 9.4% within 30 min of treatment using high-frequency and low-intensity ultrasounds. In summary, this method showed that low frequencies of ultrasonic devices were capable of manufacturing Fe 3 O 4 @MWCNTs through a simple and fast method.
Due to the strong influence of the nanoparticle size on the magnetic and structural properties of Fe 3 O 4 NPs, the size selection in proportion to the desired magnetization of these particles is very significant. Boustani et al. successfully demonstrated the synthesis of Fe 3 O 4 NPs by ultrasonic treatment (40 kHz, 150 W) and a novel precipitating agent (ethylenediamine) by the coprecipitation way [54]. It was found that ethylenediamine produces Fe 3 O 4 NPs with a larger size and desired magnetization saturation (Ms). In another study, a single, inexpensive and nontoxic metal salt (FeSO 4 .7H 2 O) reactant was used in aqueous media to synthesize monodisperse Fe 3 O 4 nanocubes with a uniform particulate size of about 80 nm using the sonochemical method [55]. The magnetic properties of Fe 3 O 4 nanocubes demonstrated a magnetization of 91 emu/g for the as-synthesized sample at 5 K and of 94.8 emu/g for the sample that was annealed by a vacuum chamber at 600 • C. Due to high magnetization, these nanoparticles can be used for various applications, such as MRI and drug delivery.

AuNPs
Over the past decades, nanomaterials, especially AuNPs, have attracted a great deal of attention from the research community because of their different and unique physical, chemical, photochemical, electronic and optical properties, which also differ from the material properties in their bulk states [56][57][58]. The unique characteristics of AuNPs include high stability and chemical stability, high surface area-to-volume ratios and a surface plasmon resonance (SPR) effect [59][60][61][62]. AuNPs are also biologically unreactive, biocompatible and can be used with pharmaceutical drugs, proteins and enzymes [63]. For this purpose, they can be used in diverse medical applications, such as sensors and biosensors [64], tissue imaging [65], therapeutic agents [66], dentistry [67,68], catalysts [69], diagnosis treatment [70] and drug and gene delivery [71].
Recently, several methods of synthesis AuNPs have been developed to determine the physical and chemical properties of AuNPs by their surface structures, purity, size and morphology [72,73]. These methods are: (i) pyrolysis processes [74], (ii) flame spray synthesis [75], (iii) atomic (iv) layer deposition [76] and (v) chemical vapor deposition [77]. AuNPs can be synthesized from molecular components (metal ions) using the abovementioned methods. All these approaches are suitable for producing small amounts of AuNPs, the shapes and sizes of which depend on the batch used. Sonochemical is a great potential method for AuNP mass production from different materials. This method is a relatively powerful and straightforward technique for producing nanomaterials, and it is possible to control the properties of nanoparticles by modifying the parameters of the ultrasonic process [78,79]. AuNPs with semispherical shapes and average size distributions of about 18.5 were produced through an economical sonochemical method in which the nanoparticles were produced with ultrasounds from droplets of the metal salt precursor solution ( Figure 2) [80]. The sonicator probe model (SONICS Ultra-cell MODEL: VC 750) operated for synthesis has an output power, frequency and tip size of 17.9 W·cm 2 , 20 kHz and half an inch, respectively. Under ultrasound waves of 5 min, AuNPs showed high stability in different media (AuNPs in phosphate-buffered saline and water were −39.5 mV and −42.1 mV, respectively). The homogeneity of AuNPs may also be attributed to the intense power and high energy produced by ultrasonic irradiation during the formation and collapse of bubbles, which increase the pressure and temperature of the solution.  Yasuda et al. synthesized AuNPs by ultrasonic irradiation at 495 kHz from aqueous solution HAuCl 4 without reducing the agent or surfactant [81]. The ratio of spherical AuNPs increased with the introduction of ultrafine bubbles (UFBs), and the average diameter of the spherical AuNPs reduced from 119 nm to 22 nm. The reduction of the Au ion was hypothesized to be accelerated by UFBs, because UFBs were nuclei of ultrasonic cavitation, which increased cavitation generation. In addition, AuNP synthesis with UFBs seemed to be stable in the solution, because the AuNPs were immobilized onto UFBs electrostatically, and the lifetimes of UFBs in the liquid were very long. During the pulseon time, the cavitation and AuNP nucleation improved, whereas, with increasing the pulse-off time, the mean diameter also increased. The AuNPs developed during the pulseoff time. AuNP size regulation in the absence of reducing agents and surfactants was effective by optimizing the number of UFBs and the pulsed ultrasonic conditions. Kumar et al. reported a simple sonochemical method for the preparation of gold-ruthenium (Au-Ru NPs) by co-reduction, and sequential reduction methods were developed [82]. Nanoparticles have the potential for being used in direct methanol fuel cells as catalysts in electrode materials. In addition, the preparation of Au-Ru NPs covered by a polymer was systematically investigated by TEM and a UV-vis spectral study. During the reduction of metal ions, the UV-vis spectral findings suggest that their redox potential governs the order of the reduction process (metal ions), i.e., Au is first reduced, accompanied by ruthenium. Additionally, AuNPs serve as an electron sink to reduce the time needed for Ru 3+ reduction significantly from 7 h to 4 h. Cui et al. demonstrated that hybrid AuNPs wrapped graphene oxide (GO) materials can be designed and self-assembled through a one-pot sonochemical reaction using HAuCl 4 and GO precursors [83]. The morphology of the composite materials obtained is that of the AuNP spheres covered with GO sheets like gauze. It is important to use ethylene glycol to synthesize AuNPs, because it is nontoxic. In addition, Au NPs exhibit excellent surface-enhanced Raman scattering in hybrid materials and have also been reported to improve enhanced photocatalytic activity through light irradiation. This method provides a simple way of controlling and tuning the morphology and size of Au NPs in GO-wrapped metal nanoparticles, which expands as a feasible way to produce metal NPs/GO composites employing GO as the precursor material. Wang et al. documented a method of preparing fabrics that can prevent biofilm formation by sonochemical decoration AuNPs covered with N-heterocyclic molecules [84]. Since N-heterocyclic molecules and AuNPs are not toxic to mammalian cells, their research offers a novel strategy to superb antimicrobial activity against multidrug-resistant (MDR) biofilm bacteria in a simple, low-cost and effective manner that holds promise for wide clinical applications. The sonochemical production of AuNPs is recorded utilizing a high-intensity ultrasound (HIU) performing at 463 kHz with various shapes and size distributions [85]. AuNPs are formed by reducing Au 3+ to Au 0 by radicals produced through acoustic cavitation. The TEM images revealed that AuNPs exhibit irregular shapes at 30 W, are predominantly icosahedral at 50 W and contain a large amount of 70-W nanorods. AuNP sizes decrease with a narrower size distribution, with increasing acoustic power. The number of radicals formed and the mechanical forces produced control the AuNP size and shape. The TEM images and UV-Vis spectra can be used to indicate a potential explanation for the results observed. The results show that the HIU process can be used to synthesize size-and shape-controlled metal nanoparticles. Radziuk et al. demonstrated that ultrasonic irradiation (20 kHz) for 20 min is enough to fuse the AuNPs in a dumbbell-like structure at the contact [86]. After 60 min of sonication in water, AuNPs acquire a ring-like or worm-like structure. Fused AuNPs with oval or spherical shapes with a size of about 25 nm forms in the presence of dodecyl amine solutions or sodium dodecyl sulfate after ultrasonic irradiation. The dispersion of AuNPs, which is the weakest in pure water, is found as an additional cycle during sonication. The results reported might be of interest to the ultrasonic melting of inorganic materials at the nanoscale to produce metal structures with different properties and morphologies. Recently, by our team, AuNPs with different output powers have been synthesized (A1 = 12, A2 = 20 and A3 = 36 W) [87]. Figure 3 confirms the influence of ultrasounds on the synthesis of various AuNPs as a feature of ultrasound control. The typical diffraction peaks of Au are visible in all samples, but the intensity of the prominent (111) peak for Au is greater at 36 W. This result suggests that the structural properties of the synthesized AuNPs were affected by the output power, as the samples displayed significant differences in peak intensities as the output power was increased. The comparison of the various spectra found that the peak amplitude improved as the ultrasound output power increased. This phenomenon may be due to the distinct characteristics derived from the acoustics.
like structure at the contact [86]. After 60 min of sonication in water, AuNPs acquire a ring-like or worm-like structure. Fused AuNPs with oval or spherical shapes with a size of about 25 nm forms in the presence of dodecyl amine solutions or sodium dodecyl sulfate after ultrasonic irradiation. The dispersion of AuNPs, which is the weakest in pure water, is found as an additional cycle during sonication. The results reported might be of interest to the ultrasonic melting of inorganic materials at the nanoscale to produce metal structures with different properties and morphologies. Recently, by our team, AuNPs with different output powers have been synthesized (A1 = 12, A2 = 20 and A3 = 36 W) [87]. Figure 3 confirms the influence of ultrasounds on the synthesis of various AuNPs as a feature of ultrasound control. The typical diffraction peaks of Au are visible in all samples, but the intensity of the prominent (111) peak for Au is greater at 36 W. This result suggests that the structural properties of the synthesized AuNPs were affected by the output power, as the samples displayed significant differences in peak intensities as the output power was increased. The comparison of the various spectra found that the peak amplitude improved as the ultrasound output power increased. This phenomenon may be due to the distinct characteristics derived from the acoustics.

Fe3O4@AuNPs
Recently, many achievements and scientific outcomes in nanotechnology have contributed to the creation of nanomaterials with the desired structure, chemical and physical compositions [88][89][90][91].There is currently increasing interest in nanomaterials with multifunctional properties that can be produced for different tasks. Specifically, core-shell nanostructures are increasingly attracting attention because of their universal structures and compositions [92]. The interaction between the shell and core can lead to completely

Fe 3 O 4 @AuNPs
Recently, many achievements and scientific outcomes in nanotechnology have contributed to the creation of nanomaterials with the desired structure, chemical and physical compositions [88][89][90][91]. There is currently increasing interest in nanomaterials with multifunctional properties that can be produced for different tasks. Specifically, core-shell nanostructures are increasingly attracting attention because of their universal structures and compositions [92]. The interaction between the shell and core can lead to completely new collective properties in a nanostructure [93,94]. Different organic and inorganic substances can be used as materials for nanostructures' shells and cores to achieve different effects and physical properties [95]. The differences in the materials used for core-shell nanostructures and, subsequently, their physical characteristics can make use of a new class of nanomaterials with a wide range of applications (e.g., bio-nanotechnology, magnetic devices, nano optics and nanomedicine) [96][97][98][99]. Core-shell nanostructures can be produced by a two-step sequential reaction in which, first, the core is formed and, then, the shell is made up [100]. Fe 3 O 4 @Au (core@shell) is one of the most significant nanoparticles used for many biomedical applications, including catalysis [101], biosensing [102], targeted drug delivery [103], phototherapy [104] and (CT/MRI) dual-modality [105]. Various methodologies were used to synthesize the Fe 3 O 4 core coated with an Au shell. For instance, direct coating is easy but requires a complicated method of combining two incompatible surfaces. The outcome typically indicates low dispersion and, therefore, fails to synthesize Fe 3 O 4 @Au NPs [106]. In addition, the procedure is time-consuming and laborious [107], as well as produces irregularly shaped and large sizes more than 100 nm, leading to an undesired impact on their medical applications [108]. To successfully synthesize correctly sized and consistently shaped Fe 3 O 4 @Au NPs through a straightforward method remains challenging. A procedure for producing Fe 3 O 4 @Au NPs with outstanding physicochemical characteristics has to be established. The sonochemistry strategy has the ability to develop into an invaluable tool for Au shell deposition on Fe 3 O 4 NPs (Figure 4). The sonochemical procedure influences the surface and structure of Fe 3 O 4 NPs through the acoustic cavity, which inhibits cluster agglomeration and leads to a more stable distribution [32]. compatible surfaces. The outcome typically indicates low dispersion and, therefore, fails to synthesize Fe3O4@Au NPs [106]. In addition, the procedure is time-consuming and laborious [107], as well as produces irregularly shaped and large sizes more than 100 nm, leading to an undesired impact on their medical applications [108]. To successfully synthesize correctly sized and consistently shaped Fe3O4@Au NPs through a straightforward method remains challenging. A procedure for producing Fe3O4@Au NPs with outstanding physicochemical characteristics has to be established. The sonochemistry strategy has the ability to develop into an invaluable tool for Au shell deposition on Fe3O4NPs (Figure 4). The sonochemical procedure influences the surface and structure of Fe3O4NPs through the acoustic cavity, which inhibits cluster agglomeration and leads to a more stable distribution [32]. Fe3O4@Au NPs have been produced to combine the features of Fe3O4 NPs and Au NPs with one core@shell nanoparticle [109]. Fe3O4 NPs were prepared by coprecipitation proceeded by a reduction of the Au shell on the Fe3O4 surface using a fast and simple sonochemical process within 10 min. Fe3O4@Au were prepared by employing sodium citrate as a both reducing and capping agent, owing to the inclusion of carboxylate ions and then identified by several methods that verified the development of the Au shell on the Fe3O4 surface. Figure 5 provides TEM images of Fe3O4NPs and Fe3O4 after being coated by AuNPs. SPR peaks shifted from 521 nm to 541 nm, indicating that the Au NPs shell is tightly adsorbed to the Fe3O4 surface. Sonochemically produced Fe3O4@Au NPs have high magnetization saturation values even after being coated with an Au shell. The high energy generated by ultrasonic irradiation enhances the covalent interaction between the core of Fe3O4 and the Au shell, even though the synthesis period was especially short. In addition, the obtained Fe3O4@Au NPs showed good biocompatibility and high transverse relaxation, as well as X-ray attenuation values, which were higher than those recorded for NPs provided by conventional approaches and commercial NPs.

Fe 3 O 4 @Au NPs have been produced to combine the features of Fe 3 O 4 NPs and Au
NPs with one core@shell nanoparticle [109]. Fe 3 O 4 NPs were prepared by coprecipitation proceeded by a reduction of the Au shell on the Fe 3 O 4 surface using a fast and simple sonochemical process within 10 min. Fe 3 O 4 @Au were prepared by employing sodium citrate as a both reducing and capping agent, owing to the inclusion of carboxylate ions and then identified by several methods that verified the development of the Au shell on the Fe 3 O 4 surface. Figure 5 provides TEM images of Fe 3 O 4 NPs and Fe 3 O 4 after being coated by AuNPs. SPR peaks shifted from 521 nm to 541 nm, indicating that the Au NPs shell is tightly adsorbed to the Fe 3 O 4 surface. Sonochemically produced Fe 3 O 4 @Au NPs have high magnetization saturation values even after being coated with an Au shell. The high energy generated by ultrasonic irradiation enhances the covalent interaction between the core of Fe 3 O 4 and the Au shell, even though the synthesis period was especially short. In addition, the obtained Fe 3 O 4 @Au NPs showed good biocompatibility and high transverse relaxation, as well as X-ray attenuation values, which were higher than those recorded for NPs provided by conventional approaches and commercial NPs. Spherical Fe3O4@AuNPs were successfully produced as a photothermal agent with a mean size of 20.8 nm by a sonochemical process [104]. At 40 kHz (ultrasound frequency), 5-mg Fe3O4NPs were ultrasonically dispersed for 15 min in 20 mL of sodium citrate. Subsequently, a freshly formulated HAuCl4 (10 mL, 0.1 M) solution was applied in order to minimize HAuCl4 and shape the shell based on Fe3O4. The process of sonication pro- Spherical Fe 3 O 4 @AuNPs were successfully produced as a photothermal agent with a mean size of 20.8 nm by a sonochemical process [104]. At 40 kHz (ultrasound frequency), 5-mg Fe 3 O 4 NPs were ultrasonically dispersed for 15 min in 20 mL of sodium citrate. Subsequently, a freshly formulated HAuCl 4 (10 mL, 0.1 M) solution was applied in order to minimize HAuCl 4 and shape the shell based on Fe 3 O 4 . The process of sonication proceeded for 15 min. A permanent magnet was used for collecting Fe 3 O 4 @AuNPs and washed thoroughly with distilled water and re-dissipated in distilled water. The Fe 3 O 4 @AuNPs cell viability assessment showed that MCF-7 lines have negligible toxicity, even with high levels of NPs, after 24 h. After illumination with a laser at 808 nm (200 mW, 10 min), MCF-7 cells treated with Fe 3 O 4 @ Au NPs were significantly reduced (73.9%) at 50-µgFe/mL viability. In this paper, results agree that the produced Fe 3 O 4 @AuNPs that pose a threat to human health could be used to increase breast cancer treatment as a photothermal therapist. The synthesis of Fe 3 O 4 @AuNPs and variations of the parameters were also further optimized using the surface response method (RSM) approach [110]. Experimental sequences of 14 different variations in sonication amplitude, sodium citrate and HAuCl 4 concentrations were performed using RSM to optimize the experimental conditions, and a variance analysis (ANOVA) was used to achieve the optimum parameters for the experimental results. The target of the zeta potential of −46.125 mV was obtained with an optimum sonication amplitude of 40%, 30 mL of sodium citrate and 10 mL of HAuCl 4 , which was consistent (about 99.2%) with the actual average of zeta potential (−45.8 mV). The results confirmed that the sonochemical method effectively synthesized monodispersed and highly stable Fe 3 O 4 @Au NPs with an average size diameter of 20 nm in less than 8 min. Figure 6 shows the TEM images of  Figure 7b. The Au shell thickness was around 11 nm and could be changed by various experimental conditions [111].  [110]. Copyright 2020 Elsevier.   [110]. Copyright 2020 Elsevier.
Another sonochemical method for developing Fe3O4@Au NPs was implemented by synthesizing Au layers on the Fe3O4 surface, with sodium citrate being used as a reductant [112]. The TEM images showed that both Fe3O4 and Fe3O4@Au NPs are highly uniformly spherical [113]. The mean diameter ranges were approximately 9 nm and 27 nm for Fe3O4NPs and Fe3O4@Au NPs, respectively. The Au shell was about 9 nm thick. The thickness of the shell can be modified by adjusting the experimental parameters [114]. Hu et al. reported that a simple but effective method (ultrasonic process (40 kHz, 50 W)) was used to produce Au-coated Fe3O4 with polyphosphazene (PZS) as a mediator [115]. PZS is an appropriate layer of glue, because it has phenolic hydroxyl groups. Fe3O4NPs were prepared under high temperatures from the iron salt precursor compound with polyol medium triethylene-glycol using ultrasonic power to irradiate a combination of hexachlorocyclotriphosphazene, triethylamine and Fe3O4. Thereafter, PZS was added to the mixture, then irradiated about 6 h; any adverse effect of long-time irradiation was not mentioned by the authors. The Fe3O4NPs-PZS were then mixed in a HAuCl4 solution under room temperature. After 30 min of ultrasonic waves, sodium citrate was added to the mixture. Another sonochemical method for developing Fe 3 O 4 @Au NPs was implemented by synthesizing Au layers on the Fe 3 O 4 surface, with sodium citrate being used as a reductant [112]. The TEM images showed that both Fe 3 O 4 and Fe 3 O 4 @Au NPs are highly uniformly spherical [113]. The mean diameter ranges were approximately 9 nm and 27 nm for Fe 3 O 4 NPs and Fe 3 O 4 @Au NPs, respectively. The Au shell was about 9 nm thick. The thickness of the shell can be modified by adjusting the experimental parameters [114]. Hu et al. reported that a simple but effective method (ultrasonic process (40 kHz, 50 W)) was used to produce Au-coated Fe 3 O 4 with polyphosphazene (PZS) as a mediator [115]. PZS is an appropriate layer of glue, because it has phenolic hydroxyl groups. Fe 3 O 4 NPs were prepared under high temperatures from the iron salt precursor compound with polyol medium triethylene-glycol using ultrasonic power to irradiate a combination of hexachlorocyclotriphosphazene, triethylamine and Fe 3 O 4 . Thereafter, PZS was added to the mixture, then irradiated about 6 h; any adverse effect of long-time irradiation was not mentioned by the authors. The Fe 3 O 4 NPs-PZS were then mixed in a HAuCl 4 solution under room temperature. After 30 min of ultrasonic waves, sodium citrate was added to the mixture. As a result, the Fe 3 O 4 -PZS-Au NPs could become an excellent candidate for photothermal therapy, as well as other applications, due to the characteristics of the Au shell.
Aziz et al. showed a simple procedure to produce Fe 3 O 4 @Au NPs using ultrasonic power that requires a chemical reduction in the existence of APTES ((3-aminopropyl) triethoxysilane)-coated Fe 3 O 4 NPs seeded through chilled sodium borohydride [116]. The acoustic cavitation effect provides high pressure and high thermal energy. On the Fe 3 O 4 surface, the Au NPs establish a covalent connection to the terminal amine. The creation of Au-coated Fe 3 O 4 NPs is stated by a change in the color of the combination to dark purple [107,117]. The observable purple color can be related to the purple or red-to-blue change in Au NP surface plasmon resonance (SPR), which is attributable in turn to Au NP conjugation with Fe 3 O 4 . Furthermore, Fe 3 O 4 @Au NPs of quite high saturation magnetization were synthesized with an easy and rapid sonochemical process (60 kHz). In the following sequence, the synthesis involved three-phase reactions: (i) producing Fe 3 O 4 NPs via the co-precipitation technique (ii), coated Fe 3 O 4 by the amine group and (iii) Au 3+ ion reductions with the assistance of sonication waves [37]. Chemically, the ultrasound influences the activity of the nanoparticle surface through acoustic cavitation. Unlike the regular stirring method, the ultrasound method is valuable in obtaining a uniform shape, removing the variables of localized conditions, speeding up the reaction rate and developing a new phase. This procedure also reveals a shearing effect for agglomeration, which is important for high monodispersity nanoparticle synthesis. Fe 3 O 4 @Au NPs were synthesized ultrasonically with an average diameter about 9-25 nm as a stationary phase with high dispersibility, magnetic responsivity and excellent water solubility. After that, bovine serum albumin (BSA) was grafted on the Fe 3 O 4 @Au NPs surface by conjugating Au NPs with BSA to produce Fe 3 O 4 @Au NPs-BSA [118]. Fe 3 O 4 @Au-BSA have a high magnetization that enables them to be activated easily through an external magnetic field, as well as a large area and excellent biocompatibility of the Au shell. Fe 3 O 4 @Au NPs-BSA has developed a new approach in addition to novel applications of magnetic NPs in studies of large concentrations of protein target enantiomers. All in all, the results confirm that the use of sonochemical for the production of metal nanostructures provides highly stable, eco-friendly and cost-effective particularly nontoxic nanoparticles with good morphology and high-quality crystal structures [80].

Shapes of Synthesis Nanomaterials Sonochemically
Study groups around the world have, over the years, obtained nanoproducts with unusual shapes, such as nanorods, nanotubes, sphere, non-sphere, nano-hexagonal and others. This section will clarify the capacity of the sonochemical method to generate a variety of shapes for nanoparticles. Wani and Ahmad produced polyhedral structures and nanodiscs of AuNPs through the sonochemical technique without any stabilizer (Figure 8a) [119]. Sodium borohydride was used as a reducing agent and has the potential to produce a mixture of nanocrystals of various morphologies, including hexagons, cubes and other polyhedral forms with an average size of 30 nm (Table 2). Moreover, Jung et al. developed nano-cubic C-Fe 2 O 3 @Au sonochemically [120]. The Fe 2 O 3 @Au cubic is formed by applying ultrasound waves to both C-Fe 2 O 3 and HAuCl 4 . Au-coated C-Fe 2 O 3 was produced under ultrasonic irradiation (300 W, 20 kHz) for 30 min without any supporting agents. The precipitate was obtained at 8000 rpm by centrifugation and washed with distilled water three times to remove the residual impurities. The sonochemistry method provided a direct synthesis technique for the hematite cubic form decorated with nanosized Au, suggesting possible applications for lithium storage materials, catalytic support and water-splitting. A new type of nanocube with a size of about 43 nm was produced sonochemically in 30 min (Figure 8b) [121]. The sonochemical formation of Fe 3 O 4 NPs does not require strict experimental procedures or any toxic agent, and therefore, it is a fast, green, efficient and straightforward method to produce extremely active catalysts for the treatment of environmental pollutants. fast due to the high active surface area and an adsorbent vacant site that enhances the interface and a driving force. In addition, the results of this study encourage research and industry to use ultrasound devices for more efficient synthesizing nanomaterials. Takahashi et al. demonstrated an easy and effective post-modification pathway was developed to modify the surface charge of AuNPs using surfactant-free (thioctic acid) AuNPs produced via the sonochemical method [125]. The AuNPs have been synthesized in 30 min by a sonochemical surfactant-free reaction with ultrasound at 430 kHz. SEM images verified that nano spherical of AuNPs (15-20 nm) was formed during the sonication of a 200-μM HAuCl4 aqueous solution. It has been found that the presence of trace nereistoxin might cause AuNPs aggregation if thioctic acid was partially covered at pH 5 on the AuNPs surface. Since the aggregation could not have been produced without thiol groups by the other amine compounds, it showed that the pronounced nereistoxin concentration might reduce the thioctic acid surface charge covered AuNPs resulting in aggregation. A simplistic liquid-liquid reverse extraction method has been successfully used to prove the ability of the proposed method for detecting trace levels of nereistoxin in environmental water samples.

Conclusions
Sonochemistry demonstrates the use of modern methods and techniques and has proven to be more simple and rapid in some ways than mature and conventional ones for synthesizing Fe3O4, Au and Fe3O4@Au NPs. With simple alterations of the precursor compositions and reaction conditions, the usage of a high-intensity ultrasound has effectively prepared a multitude of nanostructured materials for controlled structures, morphologies and compositions. Using such exceptional conditions, naturally presented by acoustic bubbles, a large variety of nanomaterials were sonochemically synthesized even without the assistance of extensive and costly equipment or facilities. Sonochemistry helps to eliminate the complexity and to improve the handling of materials. The sonochemical method  The mechanism by which sonochemically the nanorods are formed is much simpler. Okitsu et al. reported a rapid sonochemical route (one-pot synthesis) for the production gold nanorods in the aqueous solution in the existence of ascorbic acid, silver nitrate and cetyltrimethylammonium bromide in a short time [122]. The role of time, concentration, sonication time and capping agent as effective variables has been investigated for the formation of gold nanorods via the sonochemical route. TEM image shows the histogram of the rods diameter of gold was about of 34 nm (Figure 8c). In growth investigations of gold seeds formed by sonochemistry, the induction time before growth began has been longer for shorter periods of irradiation. The result showed that the number of gold seeds that were formed by sonochemistry increased with an increase in irradiation time. The gold nanorods provided were wider and longer when the time of irradiation time was shorter. Nagvenkar et al. and Mohammadi et al. have also demonstrated the potential for fabrication nanorods in inorganic nanoparticles using the sonochemistry method [126,127].
In the case of spherical shape, Davino et al. employed the sonochemical method to prepare 9-11 nm spheres Fe 3 O 4 NPs with excellent physicochemical properties in 12 min (Figure 8d) [123]. A two-step synthesis with an ultrasound probe with a frequency of (585 W, 20 kHz) was used to synthesize and conjugate Fe 3 O 4 NPs. In addition, even with the overlay with a non-magnetic material, the sonochemistry approach generated Fe 3 O 4 NPs with high magnetization values about 77 emu/g. The high energy generated by ultrasound waves allowed the covalent bonding between the Fe 3 O 4 and capping agent molecules, given the relatively short time used during the synthesis. Fe 3 O 4 NPs coated with amine and carboxylate displayed strong colloidal stability in water which makes them promise for in vivo applications. In particular, the procedure used here overcomes the current synthesizing-related limitations of biomedical research on Fe 3 O 4 NPs from the bench to the clinics. It offers a simple experimental treatment that may bring new opportunities for the scale-up of structured Fe 3 O 4 NPs with outstanding physicochemical features suitable for biomedical usage.
In a similar study, Nazrul Islam et al. reported a simple sonochemical procedure was introduced to synthesize the spherical Fe 3 O 4 NPs, which were effectively synthesized using cheap and non-toxic metal salts as reaction mixture [124]. It is also worth noting that TEM measurements revealed that the as Fe 3 O 4 NPs were produced to have a size distribution (11 nm) in a small range and progressive monodispersity. The measurement curve for magnetization indicates that Fe 3 O 4 NPs have superparamagnetic behavior (80 emu/g), which is very similar to the bulk value of Fe 3 O 4 . They mentioned that this approach can provide an effective and quick synthetic route for bio synthesizing Fe 3 O 4 NPs and many other applications as well. In a different study, Bagheri et al. stated that a facile sonochemical method was proposed to optimize spherical Fe 3 O 4 @AuNPs [128]. The optimum values of concentration, pH, sonication time and adsorbent weight were 26.5 mg L −1 , 4.0, 4 min, 0.25, respectively. The ANOVA revealed a strong determination coefficient (Adj-R 2 > 0.920, and R 2 > 0.972). The rapid and rapid transfer of dyes to the adsorbent surface allows for rapid balance which confirms the suitability and efficiency of ultrasonic power as a powerful wastewater treatment tool. The results indicate that the initial adsorption is very fast due to the high active surface area and an adsorbent vacant site that enhances the interface and a driving force. In addition, the results of this study encourage research and industry to use ultrasound devices for more efficient synthesizing nanomaterials. Takahashi et al. demonstrated an easy and effective post-modification pathway was developed to modify the surface charge of AuNPs using surfactant-free (thioctic acid) AuNPs produced via the sonochemical method [125]. The AuNPs have been synthesized in 30 min by a sonochemical surfactant-free reaction with ultrasound at 430 kHz. SEM images verified that nano spherical of AuNPs (15-20 nm) was formed during the sonication of a 200-µM HAuCl 4 aqueous solution. It has been found that the presence of trace nereistoxin might cause AuNPs aggregation if thioctic acid was partially covered at pH 5 on the AuNPs surface. Since the aggregation could not have been produced without thiol groups by the other amine compounds, it showed that the pronounced nereistoxin concentration might reduce the thioctic acid surface charge covered AuNPs resulting in aggregation. A simplistic liquid-liquid reverse extraction method has been successfully used to prove the ability of the proposed method for detecting trace levels of nereistoxin in environmental water samples.

Conclusions
Sonochemistry demonstrates the use of modern methods and techniques and has proven to be more simple and rapid in some ways than mature and conventional ones for synthesizing Fe 3 O 4 , Au and Fe 3 O 4 @Au NPs. With simple alterations of the precursor compositions and reaction conditions, the usage of a high-intensity ultrasound has effectively prepared a multitude of nanostructured materials for controlled structures, morphologies and compositions. Using such exceptional conditions, naturally presented by acoustic bubbles, a large variety of nanomaterials were sonochemically synthesized even without the assistance of extensive and costly equipment or facilities. Sonochemistry helps to eliminate the complexity and to improve the handling of materials. The sonochemical method has demonstrated its ability to produce diverse desired sizes and shapes of Fe 3 O 4 , Au and Fe 3 O 4 @Au NPs. This review successfully highlighted its significant contributions and progress, in addition to precise discussions on the sonochemical synthesis of nanomaterials.